Are you developing new methods or applications in instrumental analytics or material characterization? Then you have the chance to win this prestigious award with a monetary prize of € 20,000.Find out more
Pore size measurement techniques
Porous materials are found throughout nature and are important for a multitude of industrial, medical, and natural processes. For example, the pores within catalysts increase the available surface for reactions to occur. In addition, reactants and products are directed to and from active sites through the porous structure. The size of the pores present in pharmaceutical tablets directly relates to their dissolution rate. The pores that travel through a filtration membrane define the size of particles which can physically pass through and those that will be removed from a fluid stream. This article provides information on classifying pores and the most commonly used techniques to accurately measure pore diameters in materials with different pore size distributions.
Pores are the openings in solid surfaces which gases, liquids, or even foreign microscopic particles can occupy. Porous materials are made in a multitude of ways from the bottom-up to the top-down approach. The bottom-up approach builds pores from an architectural process as is the case with templated carbons or chemically arranged metal-organic frameworks (MOFs) or covalent organic frameworks (COFs). The top-down approach builds pores from non-porous materials, as in leaching/etching, sintering, or steam reforming. Both methods can be highly regulated to produce desired pore structures. Depending on the type(s) of pores present, different characterization methods or a combination of methods are used for characterization.
Pores come in a variety of sizes to address a very wide range of applications. When considering pore size, a set of standards approved by IUPAC has defined pore size ranges based on different size widths. Pores with an internal width of less than 2 nm are referred to as micropores, those with an internal width between 2 nm and 50 nm as mesopores, and those larger than 50 nm are called macropores (See Figures 2 and 3).
Within the micropore domain, there is a further subdivision into narrow micropores (ultramicropores of less than 0.7 nm) and wide micropores (supermicropores of 0.7 nm to 2 nm). These terms are used throughout different industries and in academia to easily compare and recognize material dimensions.
Pores are also defined by their accessibility to the surface of the material. A closed pore is inaccessible to its surfaces; a blind pore is accessible from the surface but does not travel completely from the upstream to the downstream surface, while a through pore travels from the upstream surface to the downstream surface of a material (See Figure 4).
How to measure pore size
Closed porosity, the overall volume of closed pores contained within a material, is estimated by comparing true density results with expectations. This technique will not provide any pore size distribution information, but an estimate of the voids within a material may be generated with the use of a gas pycnometer. Because blind pores and through pores are accessible via the material surface, techniques such as gas adsorption, mercury intrusion, and capillary flow porometry can be used for their assessment.
Gas adsorption experiments are used to characterize the surface area, pore size distribution, and pore volume of those pores accessible from the surface of porous materials. A wide range of pore sizes from 0.35 nm to over 100 nm can be analyzed with high accuracy using vacuum-volumetric or gravimetric adsorption techniques. Samples regularly evaluated using gas adsorption include zeolites, clays, activated carbons, templated materials, metal-organic frameworks, pharmaceuticals, catalysts, and many more.
These experiments are performed by first cleaning the surfaces of the sample and then dosing the sample with an adsorbing gas, in a system typically held at the boiling point of the gas (e.g., N2 at 77 K, Ar at 87 K), and recording the resulting difference in volume or mass once thermodynamic equilibrium is achieved. This dosing procedure continues over a range of predefined pressures in order to generate a characteristic isotherm (a curve of the volume adsorbed as a function of pressure created at a constant temperature, see Figure 5) which is used to determine the pore size, pore volume, and surface area. Analysis of the pore size distribution is carried out by applying different theories and calculations. Classic methods exist to determine pore size distributions, for instance:
- BJH – named for the scientists Barrett, Joyner, Helenda, it is used to describe mesopores (See Fig. 6).
- HK – named for the scientists Horvath and Kawazoe, it is generally applied to describe micropores.
However, modern methods such as DFT (Density Functional Theory) or GCMC (Grand Canonical Monte Carlo) based molecular simulations are more regularly applied. These improved data fitting methods are very reliable for siliceous/oxidic materials using non-local DFT methods and for carbonaceous materials using quenched solid DFT methods .
Measuring pores sized from 3.2 nm to larger than 400 μm accessible from the surface of a material is generally accomplished with the use of mercury intrusion porosimetry.
Pr = -2γ cosθ
r = pore radius
γ = surface tension
θ = contact angle
The pore size distribution is obtained by monitoring the volume of intruded mercury into the pores as a function of applied pressure to produce a porosimetry curve (See Figure 8).
By relating the pressure at which intrusion is seen to the size of the pore being filled, a pore size distribution plot is calculated (See Figure 9). It is important to note that for powder samples, pores may exist within particles (intraparticle pores), but always between particles (interparticle pores). Therefore, it is often important to know about the physical nature of the material being measured for proper interpretation of the results.
It is worth noting that, unlike gas adsorption, mercury intrusion porosimetry is destructive and the sample is not recoverable upon measurement.
Capillary flow porometry
If the pores of interest are through pores, to predict the performance of an ultrafiltration or microfiltration media, or simply to better understand how a material will affect fluid flow, capillary flow porometry is the more appropriate method. Capillary flow porometry is used to define through pores sized from about 13 nm to more than 500 μm. It utilizes capillary effects (attractive forces between surface and fluid) to initially hold a completely wetting fluid within the pores of a material (See Figure 10).
This technique also uses the Washburn equation, but instead of a non-wetting liquid being forced into pores, a completely wetting fluid is filled into pores and expelled as increasing pressures of gas are applied to the upstream side of the sample and the capillary forces holding the fluid in the pores are overcome. Ultimately the pore size distribution can be derived from the measurement of the resulting gas flow through the sample (See Figures 11 and 12).
Unlike gas adsorption and mercury intrusion, this technique does not quantify the pore volume, only the diameters of the through pores present in a sample; and only the smallest diameter present along the pathway of each through pore. The technique provides a means to understand how many pathways of a particular pore size exist and therefore how many particles of a certain size will be removed from a fluid stream before cleaning or replacement of the membrane must occur. Even though these pores are included in gas adsorption and mercury intrusion measurements their actual volume is oftentimes too small to be sufficiently discernible by those techniques. However, for materials containing only through pores which have uniform pore structures, such as nuclear track-etched membranes, pore size distribution results from a capillary flow porometer will be similar to gas adsorption or mercury intrusion results (depending upon the size range of the pores present).
There is a wide range of analytical methods available in the laboratory to conduct pore size analysis. To find the proper method to measure the pore size(s) within a material, it is best to consider a few factors. First, what pore size range will the materials possess? Second, is the material to be recovered? What type(s) of pores are to be measured? Finally, how representative is the measurement for the entire sample? Answering these questions will guide the user to select the best method to perform successful pore size analysis.
- Sing, S. W., Everett, D. H., Haul, R. A. W., Moscou, L., Pieroti, R. A., Rouquerol, J., Siemieniewska, T. (1985). Reporting physisorption data for gas/solid systems with special reference to the determination of surface area and porosity, Pure Appl. Chem. 57, 603
- Thommes, M., Kaneko, K., Neimar, A. V., Olivier, J. P., Rodriguez-Reinoso, F., Rouquerol, J., Sing. K. S.W. (2015). Physisorption of gases, with special reference to the evaluation of surface area and pore size distribution (IUPAC Technical Report), Pure and Applied Chemistry, Volume 87, Issue 9-10, pp 1051–1069.
- Barrett, E. P., Joyner, L. G., Halenda, P. R. (1951). The determination of pore volume and area distributions in porous substances. I. Computations from nitrogen isotherms. J. Am. Chem. Soc., 73(1), pp. 373–380
- Horvath, G., Kowazoe, K. (1983). Method for the calculation of effective pore size distribution in molecular sieve carbon. J. Chem. Eng. Jpn., 16(6), pp. 470–475.
- Washburn, E. W. (1921). Note on a method of determining the distribution of pore sizes in a porous material. Proc. Natl. Acad. Sci. USA, 7(4), pp. 115–116.